# Page History

## Key

• This line was added.
• This line was removed.
• Formatting was changed.

Reserved for Miklós Nemesszeghy

# Introduction

Rechargeable Al-ion based batteries are considered promising future electrochemical energy storage devices. As a high valence ion (+III specifically), Al-ion utilizing batteries have a potential for high energy density and capacity as each oxidation/reduction reaction transfers multiple electrons per atom/ion

DOI cite
superscript false true 10.1016/j.cej.2019.05.085
. In addition, Al is the most abundant metal in Earth's crust
DOI cite
superscript false true 10.1016/j.enchem.2020.100049
, is not harmful to the environment and the relatively small ionic radii of Al3+-ion (53 pm) is promising for intercalation chemistries
DOI cite
superscript false true 10.1016/j.cej.2019.05.085
. Some studies on Al-ion batteries were published already back in the 1900s, but large interest in the subject has emerged only recently (around 2015) to replace Li-ion batteries
DOI cite
superscript false true 10.1016/j.enchem.2020.100049
.

A typical Al-ion battery has aluminium metal foil as the negative electrode, a chloride based ionic liquid as electrolyte, and a positive electrode, supporting Al-ion intercalation. Al-ions are transported between electrodes in the electrolyte as AlCl4-- and Al2Cl7--ions. During discharge, the Al-ions intercalate into the positive electrode, while during charge, the Al-ions are plated onto the Al negative electrode.

DOI cite
superscript false true 10.1002/aenm.202002151
Figure 1 shows the working mechanism of such a Al-ion battery. With the difference of intercalation versus plating, the oxidization/reduction reactions at the electrodes are
DOI cite
superscript false true 10.1002/aenm.202002151
:

Mathinline
{\text{Al}+7\text{Al}\text{Cl}_4^-\left(+3\text{Cl}^-\right)\leftrightarrow4\text{Al}_2\text{Cl}_7^-+3\text{e}^-.}

There are also numerous other working mechanisms of Al-ion based batteries, emerging from different electrode and electrolyte configurations. It should also be noted that Al-ion based batteries also include the so called Al dual-ion batteries. In dual-ion batteries cation as well as anion intercalation, or deintercalation, happens simultaneously

DOI cite
superscript false true 10.1002/adfm.202010958
. Al dual-ion batteries are meant to increase the capacity, operating voltage and reduce the cost of Al-ion based batteries
DOI cite
superscript false true 10.1016/j.ensm.2017.10.001
.

Anchor
 Figure 1 Figure 1

Figure 1. Illustration of the working principle of an ionic liquid electrolyte Al-ion battery. (License: CC BY-NC 4.0)

DOI cite
superscript false true 10.1002/aenm.202002151

# Al-ion Battery Electrodes

## Positive

A good portion of the research on Al-ion batteries was directed at finding suitable positive electrodes for Al-ion intercalation. Despite the small size of the Al3+-ion, there are relatively few materials that exhibit reversible Al-ion intercalation, because of the high charge density of the trivalent ion

DOI cite
superscript false true 10.1016/j.enchem.2020.100049
DOI cite
superscript false true 10.1039/c7ta01018d
. Successful reversible intercalation was achieved by numerous types of carbon electrodes as well as some metal compounds
DOI cite
superscript false true 10.1016/j.enchem.2020.100049
, including Mo6S8
DOI cite
superscript false true 10.1021/acs.chemmater.5b01918
, VO2 and TiO2
DOI cite
superscript false true 10.1016/j.ssi.2019.115017
, amongst numerous others (despite having relatively few suitable electrode materials).

Carbon structures such as graphite, graphene and carbon nanotubes as well as other carbon based materials are amongst the most studied positive electrodes for Al-ion batteries. Graphene and graphite materials exhibits high capacity for Al-ion intercalation, a high discharge potential with metallic Al (higher than 1.7 V; in comparison a commercial Li-ion batteries exhibit typically around 3.7 V

Single cite
pages 12 false book1

Plett, Gregory L., Battery Management Systems, Volume 1 - Battery Modeling, Artech House, 2015. Retrieved from

) and a high discharge capacity due to fast diffusion of intercalation ions

DOI cite
superscript false true 10.1002/anie.201802595
DOI cite
superscript false true 10.1016/j.electacta.2016.02.144
. Graphene is considered the superior one of the two
DOI cite
superscript false true 10.1002/anie.201802595
, however, the reason is seldom addressed in literature. In addition, it is somewhat ambiguous what certain authors consider graphene and what graphite.

The ion intercalating into graphitic electrodes is not Al3+ but instead AlCl4- (with chloride based liquid ionic electrolytes) with only one electron transfer per intercalated ion

DOI cite
superscript false true 10.1038/nature14340
. Pairing graphite electrode with an Al electrode and ionic liquid electrolyte results in a dual-ion battery, where the electrolyte is also participating in the charge storage reaction
DOI cite
superscript false true 10.1016/j.electacta.2016.02.144
Figure 2 illustrates the working mechanism of such a dual-ion battery.

Anchor
 Figure 2 Figure 2

Figure 2. Illustration of the working mechanism of a Al-dual-ion battery. (License: CC BY-NC 4.0)

DOI cite
superscript false true 10.1002/aenm.202002151

The various metal compound electrodes generally exhibit two storage reactions named insertion and conversion. In insertion, either Al3+-ions or AlCl4--ions are intercalated (or inserted) into the electrode structure, while in conversion, the reaction modifies the electrode structure itself.

DOI cite
superscript false true 10.1016/j.enchem.2020.100049
Positive electrode materials exhibiting Al3+-ion intercalation include, for example, TiO2
DOI cite
superscript false true 10.1016/j.jechem.2020.03.032
, and MoS2
DOI cite
superscript false true 10.1021/acsami.8b00100
. Se doped Cu exhibits AlCl4--ion intercalation
DOI cite
superscript false true 10.1021/acsami.8b03259
, while a VOCl based material exhibits both Al3+-ion or AlCl4--ion intercalation simultaneously
DOI cite
superscript false true 10.1016/j.jallcom.2019.07.324
Figure 3 shows the crystal structure of TiO2 with the intercalation sites for Al.

Anchor
 Figure 3 Figure 3

Figure 3. (a) The crystal structure of anatase TiO2 with intercalated Al atoms. (b) The immediate surrounding of an intercalated Al atom in TiO2. Light blue represents Ti, red O and green Al. (made with VESTA and Ms Paint; based on publication

DOI cite
superscript false true 10.1016/j.jechem.2020.03.032
)

Co-Se compounds were found to exhibit Al storage through conversion reactions

DOI cite
superscript false true 10.1016/j.enchem.2020.100049
. In CoSe2 based electrodes, the Al-ions partially substitute Co in the crystal structure, meaning that Co2+-ions would be in turn dissolve into the electrolyte. In bulk CoSe2, there is little control over this process which leads to degradation of the electrode structure and thus capacity loss over time.
DOI cite
superscript false true 10.1039/c8ee00822a

In addition to the examples provided here, there are numerous other positive electrode materials under research for Al-ion batteries, including some exotic ones that can't be categorized in the above manner. Also, the examples provided are not fully investigated and may not be the best preforming solutions for an Al-ion battery positive electrode. Al-ion batteries are still in active development.

## Negative

The majority of research on Al-ion batteries has been focused on exploring electrolytes and positive electrodes and far less the possible negative electrodes. However, the widely used Al foil negative electrode has some considerable drawbacks. A metallic Al foil electrode is susceptible to dendrite growth and uneven corrosion which results in its eventual pulverization after repeated charge discharge cycles

DOI cite
superscript false true 10.1002/cey2.155
, limiting the lifetime of Al-ion battery devices.

One alternative is using an intercalation mechanism, instead of plating, at the negative electrode as well. An example would be MnO3 as negative electrode

DOI cite
superscript false true 10.1016/j.cej.2019.05.085
. Another approach includes using a highly corrosion resistant material, such as Cu foil, and use that as the basis for Al plating and stripping, eliminating the pulverization danger
DOI cite
superscript false true 10.1149/2.0131915jes
. However, this does not address the issue caused by dendrite growth. There are more examples, like TiO2 nanopowder and carbon black mixture
DOI cite
superscript false true 10.1007/s10800-018-1154-x
, and N-doped carbon nanorod array
DOI cite
superscript false true 10.1007/s12274-020-3088-y
as negative electrodes, but none of them are extensively studied yet.

It is also possible to protect the Al foil from pulverization and suppress dendrite growth by creating a protective oxide layer on the foil surface. The Al-ions have to deposit under the oxide layer, which suppresses dendrite growth and promotes a more even stripping of the Al foil. While the oxide layer is separating the electrode and electrolyte, the electrolyte can still penetrate through defects in the oxide layer. This enables a longer operating time for the Al foil electrode.

DOI cite
superscript false true 10.1021/acsami.7b07024
However, it is also reported that these protective oxide layers are corroded over time in ionic liquid electrolytes
DOI cite
superscript false true 10.1002/cey2.155
.

A novel idea for a negative electrode is using liquid Ga. As a liquid, Ga provides a uniform dendrite free surface. The Al-ions go through alloying and dealloying at the Ga electrode during charge and discharge respectively. While this material can successfully eliminate dendrite growth and other electrode degradation, a battery using this electrode material would mostly be suited for stationary applications only due to the liquid nature of the electrode.

DOI cite
superscript false true 10.1016/j.cej.2019.123594
In addition, the battery would effectively be unusable below 30οC.

# References

Cite summary
enumerationStyle [1]